2.
4 V.V. Naletov et al.
Fig. 1.1 Schematic
representation of the
experimental setup. Two
independent excitation
circuits are used: in red, the
circuit allowing the injection
of an RF current
perpendicular-to-plane
through the nano-pillar (irf,
red arrow); in blue, the circuit
allowing the generation of an
RF in-plane magnetic ﬁeld
(hrf, blue arrow)
intra or inter STNOs. It also determines the optimum strategy to couple to the auto-
oscillating mode observed when the spin transfer torque compensates the damping,
a vital knowledge to achieve phase synchronization in arrays of nano-pillars [12].
These SW modes also have a fundamental inﬂuence on the high frequency proper-
ties of spin-valve devices, and in particular on the noise of magneto-resistive sensors
[13, 14].
This work concentrates on a comprehensive identiﬁcation of the SW eigen-
modes in a normally magnetized circular spin-valve nano-pillar, where the axial
symmetry is preserved. We shall perform a comparative spectroscopic study of
the SW modes excited either by an RF current ﬂowing perpendicularly through
the nano-pillar, as used in spin-torque driven ferromagnetic resonance (ST-FMR)
[15, 16], or by a homogeneous RF in-plane magnetic ﬁeld, as used in conventional
FMR. The experimental spectra are compared to micromagnetic simulations of the
time decay response of the local magnetization to a small perturbation of the mag-
netic conﬁguration. This allows identifying and labeling the observed SW eigen-
modes, according to their symmetry and to the dipolar coupling between the two
magnetic layers.
The spin-valve structure used in this study is a standard Permalloy
(Ni80Fe20 = Py) bi-layer structure sandwiching a 10 nm copper (Cu) spacer: the
thicknesses of the thin Pya and the thick Pyb layers are respectively ta = 4 nm and
tb = 15 nm. The extended ﬁlm is patterned by standard e-beam lithography and ion-
milling techniques to a nano-pillar of radius 125 nm. The magnetic parameters of
this sample have been measured in [17], and are reported in Table 1.1. The top Cu
and bottom Au contact electrodes are shown in red in Fig. 1.1. They are impedance
matched to allow for high frequency characterization by injecting an RF current irf
through the device. Hereafter, spectra associated to SW excitations by this part of
the microwave circuit will be displayed in a red tone.
The originality of our design is the addition of an independent top microwave
antenna whose purpose is to produce an in-plane RF magnetic ﬁeld hrf at the nano-
pillar location. In Fig. 1.1, this part of the microwave circuit is shown in blue. In-
jecting a microwave current from a synthesizer inside the top antenna produces a
homogeneous in-plane linearly polarized microwave magnetic ﬁeld, oriented per-
3.
1 Spin-Wave Eigen-modes in a Normally Magnetized Nano-pillar 5
pendicularly to the stripe direction. Hereafter, spectra associated to SW excitations
by this part of the microwave circuit will be displayed in a blue tone.
We shall use in this study a method independent of transport to detect the mag-
netic resonance inside a spin-valve nanostructure: a Magnetic Resonance Force Mi-
croscope (MRFM) [18–20], hereafter named mechanical-FMR. A ﬁrst decisive ad-
vantage of the mechanical-FMR technique is that the detection scheme does not rely
on the SW spatial symmetry because it measures the change in the longitudinal com-
ponent of the magnetization. It thus probes all the excited SW modes, independently
of their phase [21, 22]. A second decisive advantage is that mechanical-FMR is a
very sensitive technique that can measure the magnetization dynamics in nanostruc-
tures buried under metallic electrodes [23]. Indeed, the probe is a magnetic particle
attached at the end of a soft cantilever and is coupled to the sample through dipolar
interaction.
The mechanical detector consists of a 800 nm diameter sphere of soft amorphous
Fe (with 3 % Si) glued to the apex of an Olympus Bio-Lever having a spring con-
stant k ≈ 5 mN/m. In our setup, the separation between the center of the spherical
probe and the nano-pillar is set to 1.3 µm (see Fig. 1.1), which is a large distance
considering the lateral size of the sample. The external magnetic ﬁeld produced by
an electromagnet is oriented out-of-plane, exactly along the nano-pillar axis ˆz. In
our study, the strength of the applied magnetic ﬁeld shall exceed the saturation ﬁeld
(≈ 8 kOe), so that the nano-pillar is studied in the saturated regime. The mechan-
ical sensor measures then the spatial average of the longitudinal component Mz of
magnetization:
Mz ≡
1
V V
Mz(r)d3
r, (1.1)
where the chevron brackets stand for the spatial average over the volume of the
magnetic body. We emphasize that for a bi-layer system, the force signal integrates
the contribution of both layers.
The experimental spectra will be shown below in Fig. 1.4(b) and Fig. 1.5(b). The
important point is that the two SW spectra excited by hrf and irf are distinct, imply-
ing that they have a different origin. It will be shown in the theoretical Sect. 1.2.1
that the RF ﬁeld and the RF current excitations probe two different azimuthal sym-
metries . Namely, only = 0 modes are excited by the uniform RF magnetic ﬁeld,
whereas only = +1 modes are excited by the orthoradial RF Oersted ﬁeld asso-
ciated to the RF current [24]. The mutually exclusive nature of the responses to the
uniform and orthoradial symmetry excitations is a property of the preserved axial
symmetry, where the azimuthal index is a good quantum number, i.e., different
-index modes are not mixed and can be excited separately.
1.2 Identiﬁcation of the Spin-Wave Modes
In this section, we discuss the boundary-value problem for SW propagation inside
normally magnetized disks, where the conﬁnement leads to a discrete SW spectrum.
4.
6 V.V. Naletov et al.
Neglecting the thickness dependence, only three indices are required to label the
resonance peaks: the usual azimuthal and radial indices for a single disk ( ,m),
plus an additional index referring to the anti-binding or binding (A or B) coupling
between the two magnetic layers in mutual dipolar interaction.
1.2.1 Single Magnetic Disk
SW eigen-modes are the solutions of the linearized equation of motion of the mag-
netization, obtained by decomposing the instantaneous magnetization vector M(t)
into a static and dynamic component [25]:
M(t)
Ms
= ˆu + m(t) + O m2
, (1.2)
where the transverse component m(t) is the small dimensionless deviation (|m| 1)
of the magnetization from the local equilibrium direction, ˆu. In ferromagnets,
|M| = Ms is a constant of the motion, so that the local orthogonality condition
ˆu · m = 0 is required.
We restrict our study to the case of thin layers so that one can assume that the
magnetization dynamics is uniform along the thickness. For a normally magnetized
disk, where ˆu = ˆz, the SW modes can be classiﬁed according to their behavior under
rotations in the x–y plane (2D vector equations with polar coordinates ρ and φ):
m =
1
2
(ˆx + i ˆy)e−i φ
ψ (ρ), (1.3)
where the functions ψ (ρ) describe the dependence of the SW mode on the radial
coordinate ρ and have to be determined from the dynamical equations of motion. To
satisfy the appropriate boundary conditions at the edges of the magnetic body [26],
we shall use as the trial vectors the radial proﬁles of the form ψ (ρ) = J (k ,nρ),
where J (x) is the Bessel function and k ,n are SW wave-numbers determined from
the pinning conditions at the disk boundary ρ = R. For our experimental conditions
(ta,tb R), the pinning is almost complete, and we shall use k ,n = κ ,n/R, where
κ ,n is the nth root of the Bessel function of the th order. The set of Bessel function
form here a complete basis in the space of vector functions m.
Figure 1.2 shows a color representation of the Bessel spatial patterns for different
values of the index ν = ,n. We restrict the number of panels to two values of
the azimuthal mode index, = 0,+1, with the radial index varying between n =
0,1,2. In our color code, the hue indicates the phase (or direction) of the transverse
component mν, while the brightness indicates the amplitude of |mν|2. The nodal
positions are marked in white. A node is a location where the transverse component
vanishes, i.e., the magnetization vector is aligned along the equilibrium axis. This
coding scheme provides a distinct visualization of the phase and amplitude of the
precession proﬁles. The black arrows are a snapshot of the mν vectors in the disk
and are all rotating synchronously in-plane at the SW eigen-frequency.
5.
1 Spin-Wave Eigen-modes in a Normally Magnetized Nano-pillar 7
Fig. 1.2 Color representation
of the Bessel spatial patterns
for different values of the
azimuthal mode index (by
row) and radial mode index n
(by column). The arrows are a
snapshot of the transverse
magnetization mν , labeled by
the index ν = ,n
The top left panel shows the ν = 0,0 ( = 0, n = 0) mode, also called the uni-
form mode. It usually corresponds to the lowest energy mode since all the vectors
are pointing in the same direction at all time. Below is the = +1, n = 0 mode. It
corresponds to SWs that are rotating around the disk in the same direction as the
Larmor precession. The corresponding phase is in quadrature between two orthog-
onal positions and this mode has a node at the center of the disk. The variation upon
the n = 0,1,2 index ( being ﬁxed) shows higher order modes with an increasing
number of nodal rings. Each ring separates regions of opposite phase along the ra-
dial direction. All these spatial patterns preserve the rotation invariance symmetry.
The coupling to an external coherent source depends primarily on the -index
[27] as the excitation efﬁciency is proportional to the overlap integral
hν ∝ mν · h1 , (1.4)
where h1(r) is the spatial proﬁle of the external excitation ﬁeld. It can be easily
shown that a uniform RF magnetic ﬁeld, h1 = hrfx, can only excite = 0 SW
modes. Obviously, the largest overlap is obtained with the so-called uniform mode
(n = 0). Higher radial index modes (n = 0) still couple to the uniform excitation
but with a strength that decreases as n increases [19, 28]. The = 0 normal modes,
however, are hidden because they have strictly no overlap with the excitation. In
contrast, the RF current-created Oersted ﬁeld, h1 = hOe(ρ)(−sinφ ˆx + cosφ ˆy) has
an orthoradial symmetry and can only excite = +1 SW modes.
1.2.2 Double Magnetic Disks
The interaction between two identical magnetic layers leads to the splitting of the
uniform mode in each layer into two collective modes: the binding and anti-binding
modes. This has been observed in interlayer-exchange-coupled thin ﬁlms [29] and
in trilayered wires where the two magnetic stripes are dipolarly coupled [30]. In the
6.
8 V.V. Naletov et al.
case where the two magnetic layers are not identical (different geometry or mag-
netic parameters), this general picture continues to subsist. Although both isolated
layers have eigen-modes with different eigen-frequencies, the collective magnetiza-
tion dynamics in each layer are still symmetrically or anti-symmetrically coupled.
But here, the precession of magnetization can be more intense in one of the two
layers and the spectral shift of the coupled SW modes with respect to the isolated
SW modes is reduced, as it was observed in both the dipolarly- [30] and exchange-
coupled cases [31].
Here, we assume that the dominant coupling mechanism between the two mag-
netic disks in the nano-pillar is the dipolar interaction. We neglect any exchange
coupling between the magnetic layers mediated through the normal spacer or any
coupling associated to pure spin currents [7, 32] in our all-metallic spin-valve struc-
ture. Our nano-pillar consists of two dislike magnetic layers, having different thick-
nesses, with ta < tb, and different saturation magnetizations, with Ma < Mb. In the
normally saturated state which is considered here, this difference of magnetization
leads to a difference in the internal demagnetizing ﬁeld of each layer (self dipolar
coupling) and in the stray ﬁeld of one layer on the other one (cross dipolar coupling).
As a result, the eigen-frequency of the uniform mode of the thin layer is larger than
the one of the thick layer, ωa > ωb. This is represented in Fig. 1.3(a), on both sides
of the bi-layer diagram, where we have reported on an energy scale their relative
positions.
In the perpendicular geometry, the strength of the dynamical dipolar coupling
Ω between the layers depends on the cross tensor element jj , associated to the
in-plane component of the dipolar magnetic ﬁeld produced inside layer j by the
in-plane component of the magnetization of layer j (see [17, 33]). It is attractive
(lower in energy) when both layers precess in anti-phase because the dynamical
dipolar charges in each layer are alternate (anti-ferromagnetic coupling). Thus the
binding state corresponds to a collective motion where the two layers vibrate anti-
symmetrically (B) and the anti-binding state to a collective motion where they vi-
brate symmetrically (A). In this case, the larger of the frequencies (ωa) shifts up
by
ω =
Ω2
ωa − ωb
, (1.5)
while the smaller one (ωb) shifts down by the same amount. This effect is summa-
rized in Fig. 1.3.
A numerical estimate of the coupling strengths between the lowest energy SW
modes in each disk can be found in [17]. For the experimental parameters, Ω/2π
0.5 GHz. This coupling is almost an order of magnitude smaller than the frequency
splitting ωa − ωb, caused mainly by the difference of effective magnetizations of
two disks: γ 4π(Mb − Ma) 2π · 4.5 GHz. As a result, the shift of the resonance
frequencies due to the dipolar coupling is negligible, ω/2π 0.06 GHz. The
effect of dynamic dipolar interaction is more pronounced for the level of mode hy-
bridization. For instance, at the frequency ωA ≈ ωa, the ratio between the precession
7.
1 Spin-Wave Eigen-modes in a Normally Magnetized Nano-pillar 9
Fig. 1.3 Schematic representation of the coupled dynamics between two different magnetic disks.
When the two disks are dynamically coupled through the dipolar interaction, the binding state B
corresponds to the two layers oscillating in anti-phase at ωB , with the precession occurring mostly
in the thick layer, whereas the anti-binding state A corresponds to the layers oscillating in phase at
ωA, with the precession mostly in the thin layer
amplitudes in the two layers is given by
|cb/ca|ωA = ω/(γ ha,b)
Ω
ωa − ωb
. (1.6)
For the experimental parameters, Ω/(ωa −ωb) ≈ 0.1, i.e., the precession amplitude
in the disk b is about 10 % of that in the disk a. Thus, although the dipolar coupling
induces a small spectral shift (second order in the coupling parameter (1.5)), its in-
ﬂuence in the relative precession amplitude is signiﬁcant (ﬁrst order in the coupling
parameter (1.6)).
1.2.3 Micromagnetic Simulations vs. Mechanical-FMR
Experiments
Although the analytical formalism presented above allows estimating the spectrum,
several approximations have been made. In particular, we have assumed total pin-
ning at the disks boundary for the SW modes and no variation of the precession
proﬁle along the disks thicknesses (2D model), and we have neglected the depen-
dence on the mode index ν of the dynamic dipolar coupling. Instead of developing
a more complex analytical formalism, we have performed a complete calculation
of the SW spectra inside our nano-pillar sample using the open source micromag-
netic simulation package Nmag [34]. Nmag is a ﬁnite element solver based on the
general purpose multi-physics library Nsim. It is developed by the group of H. Fan-
gohr and T. Fischbacher in the School of Engineering Sciences at the University of
Southampton.
8.
10 V.V. Naletov et al.
Table 1.1 Magnetic parameters of the thin Pya and thick Pyb layers measured by mechanical-
FMR in the nano-pillar
4πMa (G) αa 4πMb (G) αb γ (rad s−1 G−1)
8.0 × 103 1.4 × 10−2 9.6 × 103 0.85 × 10−2 1.87 × 107
In this simulation, the full three-dimensional (3D) dynamics of the bi-layer sys-
tem is calculated. The thin layer is discretized with a mesh of 4 nm (equal to its
thickness), and the thick layer with a mesh of 3 nm. The numbers of nodes are re-
spectively 6135 in the thin layer and 37598 in the thick layer. The magnetic param-
eters introduced in the code are the ones reported in Table 1.1. The magnetization
vector is assumed to be uniform inside each cell, which is valid because the cell size
is smaller than the exchange length Λ 5 nm in Permalloy. We emphasize that the
simulations incorporate the perturbing presence of the magnetic sphere attached on
the MRFM cantilever. Moreover, the 10 nm thick Cu spacer is replaced by vacuum,
so that the layers are only coupled trough the dipolar interaction (spin diffusion
effects are absent).
The ﬁrst step is to calculate the equilibrium conﬁguration of the normally mag-
netized nano-pillar at Hﬁx = 10 kOe. The external magnetic ﬁeld is applied exactly
along ˆz and the spherical probe with a magnetic moment m = 2 × 10−10 emu is
placed on the axial symmetry axis at a distance s = 1.3 µm above the upper sur-
face of the nano-pillar (see Fig. 1.1). The convergence criterion introduced in the
code is 1/Ms dM/dt < 1°/ns. The result reveals that the equilibrium conﬁguration
is almost uniformly saturated along ˆz. Still, a small radial ﬂaring (<5°) of the mag-
netization from ˆz is observed at the periphery of the thick and thin layers.
In order to calculate the SW spectrum corresponding to a given excitation of this
equilibrium state at Hﬁx = 10 kOe, we record the time decay response of the local
magnetization to a small perturbation of the magnetic conﬁguration, and we Fourier
transform the ringdown of the transverse magnetization [35]. Two different initial
conditions are simulated. For the conventional FMR spectrum, in which a uniform
RF ﬁeld is used to excite SW modes, we use the following perturbation vector ﬁeld:
m = ϑ
n<6
J0(k0nρ)ˆx. (1.7)
This form corresponds to an excitation which puts the same energy in the lowest
6 n-index modes with azimuthal index = 0. For the spectrum excited by an RF
current ﬂowing through the nano-pillar, which creates an orthoradial RF Oersted
ﬁeld in the magnetic volume, we use:
m = ϑ
n<6
J1(k1nρ)(−sinφ ˆx + cosφ ˆy). (1.8)
At time t = 0, we add at every mesh the perturbation vector ﬁeld deﬁned in (1.7)
or in (1.8) to the local unit vector along the equilibrium magnetization. The ﬁrst one
9.
1 Spin-Wave Eigen-modes in a Normally Magnetized Nano-pillar 11
Fig. 1.4 Panel (a) is the numerically calculated spectral response to a uniform excitation ﬁeld
h1 ∝ ˆx, from a 3D micromagnetic simulation performed at Hﬁx = 10 kOe. The peaks are labeled
according to their precession proﬁles shown in (c), (d), and (e). A light (dark) color is used to
indicate the energy stored in the thin (thick) layer. Panel (b) shows the experimental spectrum
measured by mechanical-FMR when exciting the nano-pillar by a homogeneous RF magnetic ﬁeld
at fﬁx = 8.1 GHz
corresponds to a uniform tilt (i.e., in the same azimuthal direction) of the magnetic
moments located in the center region of the two disks. The second one corresponds
to an orthoradial tilt of the magnetization at the periphery of the nano-pillar. The
perturbation angle ϑ = 0.01 1 leads to a deviation from the local equilibrium
axis of less than 1° degree, which is small enough to ensure that non-linear effects
are weak in the simulated dynamics. We then compute the magnetization decay
inside the whole sample. The ringdown of the transverse magnetization is recorded
in a 10 ns time window with a sampling interval of 5 ps.
At every time step, a spatial average of the in-plane component of the magne-
tization is recorded. In the case of the initial condition of (1.7), we construct the
complex reduced magnetization m · ˆx inside each layer j = a,b. In the case of
the initial condition of (1.8), a different spatial average is used, m · (ˆx + i ˆy)e−iφ ,
where φ is the local azimuthal coordinate of the mesh node. Then, the power density
spectrum of the time decay of the full averaged reduced magnetization is calculated
in each layer using a complex Fourier transform.
The comparison between the simulated and experimental spectra corresponding
to a uniform RF ﬁeld excitation and to an RF current ﬂowing through the nano-pillar
is presented in Figs. 1.4(a)–(b) and 1.5(a)–(b), respectively. The frequency scale of
the simulation is in correspondence with the ﬁeld-sweep scale of the experiments
10.
12 V.V. Naletov et al.
Fig. 1.5 Panel (a) is the simulated spectral response to an orthoradial excitation ﬁeld
h1 ∝ −sinφ ˆx + cosφ ˆy. Panel (b) is the experimental spectrum measured by mechanical-FMR for
an RF current excitation. Panels (c)–(e) show the simulated precession patterns of the eigen-vectors
performed at ﬁxed RF frequency fﬁx = 8.1 GHz through the afﬁne transformation
Hext − Hﬁx = 2π(f − fﬁx)/γ , as seen from the frequency and ﬁeld scales above
Fig. 1.4(a) and below Fig. 1.4(b), respectively. Since in the simulations, we have
access to the dynamics inside each layer, a light (dark) color is used to indicate the
power spectrum of the thin (thick) layer. The resonance peaks are labeled according
to the modes precession proﬁles, which are visualized by calculating the Fourier
transform of the magnetization decay at every mesh node. The results are shown
in the right side of Figs. 1.4 and 1.5, along with the precession proﬁles along the
median direction. The 2D views of the spatial distribution of the transverse magne-
tization in the thin Pya and thick Pyb layers are shown using the same color code as
in Fig. 1.2.
Let us ﬁrst focus on Fig. 1.4 which enables identifying the SW modes excited
by a uniform RF magnetic ﬁeld. The ﬁve peaks labeled on the simulated spectrum
are in correspondence with the experimental resonance peaks. From the color code
panels of Fig. 1.4(d)–(e), we see that these ﬁve modes have the same phase along the
azimuthal direction, which is the character of the = 0 index. The largest peak in
the simulation occurs at the same ﬁeld as the experimental peak at H➀. This lowest
energy mode corresponds to the most uniform mode with the largest wave-vector
and no node along the radial direction, thus it has the index n = 0. For this mode,
the thick layer is mainly precessing, with the thin layer oscillating in anti-phase, as
can be seen from the representations of its spatial proﬁle in Fig. 1.4(c), so it bears the
11.
1 Spin-Wave Eigen-modes in a Normally Magnetized Nano-pillar 13
binding index B. Therefore, it should be labeled B00, which conﬁrms the character
of the lowest energy collective mode in the perpendicular geometry discussed in
Sect. 1.2.2. We also note that the relative amplitude of the precession in the two
layers found in the simulation is roughly in agreement with the predicted value from
the analytical model, see (1.6). The same analysis can be made for the second peak,
labeled B01, which occurs close to the experimental peak at H➁. It also corresponds
to a resonance mainly in the thick layer, and its color representation shows that this is
the ﬁrst radial harmonic (n = 1), with one line of node in the radial direction. Again,
the thin layer is oscillating in anti-phase, with the same radial index n = 1, as clearly
shown by the mode proﬁle along the median direction. The third peak is labeled A00
and is located close to the experimental peak at H➂. It corresponds this time to a
uniform (n = 0) precession mainly located in the thin layer, in agreement with the
experimental analysis presented in [17]. In this mode, the thick layer is also slightly
vibrating in phase with the thin layer (anti-binding index A). The other two modes,
A01 and B02, correspond to higher radial harmonics of = 0 modes in the nano-
pillar, at H➃ and H➄. Due to the proximity between these two modes, the precession
proﬁle of the mode B02 appears somewhat hybridized with the precession proﬁle of
the mode A01. Finally, one can also check from the simulations the independence
of the precession proﬁles on the thickness (within the uncertainty of the calculated
proﬁle, which is about ±2 %). This conﬁrms the validity of the 2D approximation
and explains the performance of the analytical model [17].
Let us now turn to Fig. 1.5(b), corresponding to the spectroscopic response to an
RF current of same frequency 8.1 GHz ﬂowing perpendicularly through the nano-
pillar. The SW spectrum is acquired under the exact same conditions as for standard
FMR, i.e., the spherical magnetic probe of the mechanical-FMR detection is kept
at the same location above the sample. The striking result is that the position of the
peaks in Figs. 1.4(b) and 1.5(b) do not coincide. More precisely, there seems to be
a translational correspondence between the two spectra, which are shifted in ﬁeld
by about 0.5 kOe from each other. The comparison with Fig. 1.5(a) enables us to
identify the SW modes excited by the orthoradial RF Oersted ﬁeld produced by the
RF current. Here again, the peaks of the simulated power spectrum in Fig. 1.5(a)
are in good correspondence with the experimental resonance peaks in Fig. 1.5(b).
Repeating the same analysis as above, the peaks follow the same sequence of A/B,
n indexation and only differ by their -index. This explains the translational corre-
spondence between the SW spectra of Figs. 1.4(b) and 1.5(b). Finally, we point out
that the dipolar pinning at the boundaries of each disk in the modes displayed in
Fig. 1.5(c) is not trivial [36]. The general trend observed here is that the thin layer
is less pinned than the thick layer for symmetric modes, and vice versa.
Thus, these full 3D micromagnetic simulations allow the identiﬁcation of the
SW modes probed experimentally by both a uniform RF magnetic ﬁeld and an RF
current ﬂowing through the nano-pillar, i.e., of their respective selection rules. They
also give a deeper insight on the collective nature of the magnetization dynamics in
the nano-pillar discussed in Sect. 1.2.2.
12.
14 V.V. Naletov et al.
1.3 Conclusion
In summary, we used the MRFM technique [20] to study the SW eigen-modes in the
prototype of a STNO – a normally magnetized nano-pillar composed of two mag-
netic layers in dipolar interaction. We were able to compare the SW spectra of this
passive STNO excited by a uniform in-plane RF magnetic ﬁeld and by an RF cur-
rent ﬂowing perpendicularly through the layers. We found that distinctly different
SW modes (having azimuthal indices = 0 and = +1, respectively) are excited
by the two above mentioned excitation methods. We also developed a simple an-
alytic theory providing a comprehensive labeling of all the SW eigen-modes of a
magnetic nano-pillar in the studied axially symmetric case. This labeling requires
three independent indices: the usual azimuthal and radial indices and n used for
the SW modes of a single magnetic disk, and an additional index referring to the
binding or anti-binding (B or A) dipolar coupling between the two magnetic disks.
The obtained experimental and analytic results were also compared to the results
of 3D micromagnetic simulations obtained with the Nmag package. We learned that
the -index, related to the azimuthal symmetry of the SW modes, is the discriminat-
ing parameter for the selection rules of the SW mode excitation. We believe that our
results are important for the optimization of the characteristics of nano-spintronic
devices, and in particular STNOs, and for the experimental determination of the
STNO parameters.
Acknowledgements We thank V. Cros, J. Grollier, H. Hurdequint, C. Ulysse, G. Faini,
V.S. Tiberkevich, and A.N. Slavin for their help and support. This research was partially supported
by the European Grant Master (NMP-FP7 212257) and by the French Grant Voice (ANR-09-
NANO-006-01).
References
1. S. Wolf, D.D. Awschalom, R.A. Buhrman, J. Daughton, S. von Molnar, M.L. Roukes,
A.Y. Chtchelkanova, D.M. Treger, Science 294, 1488 (2001)
2. M.N. Baibich, J.M. Broto, A. Fert, F.N.V. Dau, F. Petroff, P. Etienne, G. Creuzet, A. Friederich,
J. Chazelas, Phys. Rev. Lett. 61(21), 2472 (1988)
3. G. Binasch, P. Grunberg, F. Saurenbach, W. Zinn, Phys. Rev. B 39(7), 4828 (1989)
4. J. Slonczewski, J. Magn. Magn. Mater. 159, L1 (1996). doi:10.1016/0304-8853(96)00062-5
5. L. Berger, Phys. Rev. B 54(13), 9353 (1996)
6. V.E. Demidov, S.O. Demokritov, B. Hillebrands, M. Laufenberg, P.P. Freitas, Appl. Phys.
Lett. 85(14), 2866 (2004). doi:10.1063/1.1803621
7. G. Woltersdorf, O. Mosendz, B. Heinrich, C.H. Back, Phys. Rev. Lett. 99(24), 246603 (2007).
doi:10.1103/PhysRevLett.99.246603
8. G. de Loubens, V.V. Naletov, O. Klein, J. Ben Youssef, F. Boust, N. Vukadinovic, Phys. Rev.
Lett. 98(12), 127601 (2007)
9. G. de Loubens, V.V. Naletov, M. Viret, O. Klein, H. Hurdequint, J. Ben Youssef, F. Boust,
N. Vukadinovic, J. Appl. Phys. 101, 09F514 (2007)
10. G. Gubbiotti, M. Madami, S. Tacchi, G. Carlotti, H. Tanigawa, T. Ono, J. Phys. D, Appl. Phys.
41(13), 134023 (2008). doi:10.1088/0022-3727/41/13/134023
11. P.S. Keatley, V.V. Kruglyak, A. Neudert, E.A. Galaktionov, R.J. Hicken, J.R. Childress,
J.A. Katine, Phys. Rev. B 78(21), 214412 (2008). doi:10.1103/PhysRevB.78.214412
13.
1 Spin-Wave Eigen-modes in a Normally Magnetized Nano-pillar 15
12. A. Slavin, V. Tiberkevich, IEEE Trans. Magn. 45(4), 1875 (2009). doi:10.1109/
TMAG.2008.2009935
13. A.V. Nazarov, H.S. Cho, J. Nowak, S. Stokes, N. Tabat, Appl. Phys. Lett. 81(24), 4559 (2002).
doi:10.1063/1.1521578
14. N. Stutzke, S.L. Burkett, S.E. Russek, Appl. Phys. Lett. 82, 91 (2003). doi:10.1063/1.1534386
15. J.C. Sankey, P.M. Braganca, A.G.F. Garcia, I.N. Krivorotov, R.A. Buhrman, D.C. Ralph, Phys.
Rev. Lett. 96(22), 227601 (2006)
16. W. Chen, J.M.L. Beaujour, G. de Loubens, A.D. Kent, J.Z. Sun, Appl. Phys. Lett. 92(1),
012507 (2008). doi:10.1063/1.2827570
17. V.V. Naletov, G. de Loubens, G. Albuquerque, S. Borlenghi, V. Cros, G. Faini, J. Grollier,
H. Hurdequint, N. Locatelli, B. Pigeau, A.N. Slavin, V.S. Tiberkevich, C. Ulysse, T. Valet,
O. Klein, Phys. Rev. B 84, 224423 (2011). doi:10.1103/PhysRevB.84.224423
18. Z. Zhang, P.C. Hammel, P.E. Wigen, Appl. Phys. Lett. 68, 2005 (1996)
19. V. Charbois, V.V. Naletov, J. Ben Youssef, O. Klein, J. Appl. Phys. 91, 7337 (2002)
20. O. Klein, G. de Loubens, V.V. Naletov, F. Boust, T. Guillet, H. Hurdequint, A. Lek-
sikov, A.N. Slavin, V.S. Tiberkevich, N. Vukadinovic, Phys. Rev. B 78(14), 144410 (2008).
doi:10.1103/PhysRevB.78.144410
21. G. de Loubens, V.V. Naletov, O. Klein, Phys. Rev. B 71(18), 180411 (2005)
22. V.V. Naletov, G. de Loubens, V. Charbois, O. Klein, V.S. Tiberkevich, A.N. Slavin, Phys. Rev.
B 75(14), 140405 (2007)
23. G. de Loubens, A. Riegler, B. Pigeau, F. Lochner, F. Boust, K.Y. Guslienko, H. Hurdequint,
L.W. Molenkamp, G. Schmidt, A.N. Slavin, V.S. Tiberkevich, N. Vukadinovic, O. Klein, Phys.
Rev. Lett. 102(17), 177602 (2009). doi:10.1103/PhysRevLett.102.177602
24. R.E. Arias, D.L. Mills, Phys. Rev. B 79, 144404 (2009)
25. A.G. Gurevich, G.A. Melkov, Magnetization Oscillations and Waves (CRC Press, Boca Raton,
1996)
26. K.Y. Guslienko, S.O. Demokritov, B. Hillebrands, A.N. Slavin, Phys. Rev. B 66, 132402
(2002)
27. J.F. Dillon, J. Appl. Phys. 31(9), 1605 (1960)
28. R.W. Damon, J.R. Eshbach, J. Phys. Chem. Solids 19, 308 (1961)
29. M. Belmeguenai, T. Martin, G. Woltersdorf, M. Maier, G. Bayreuther, Phys. Rev. B 76(10),
104414 (2007). doi:10.1103/PhysRevB.76.104414
30. G. Gubbiotti, M. Kostylev, N. Sergeeva, M. Conti, G. Carlotti, T. Ono, A.N. Slavin,
A. Stashkevich, Phys. Rev. B 70(22), 224422 (2004). doi:10.1103/PhysRevB.70.224422
31. J. Ben Youssef, A. Layadi, J. Appl. Phys. 108(5), 053913 (2010). doi:10.1063/1.3476269
32. B. Kardasz, O. Mosendz, B. Heinrich, Z. Liu, M. Freeman, J. Appl. Phys. 103(7), 07C509
(2008). doi:10.1063/1.2834399
33. O. Dmytriiev, T. Meitzler, E. Bankowski, A. Slavin, V. Tiberkevich, J. Phys. Condens. Matter
22, 136001 (2010)
34. T. Fischbacher, M. Franchin, G. Bordignon, H. Fangohr, IEEE Trans. Magn. 43(6), 2896
(2007)
35. R.D. McMichael, M.D. Stiles, J. Appl. Phys. 97(10), 10J901 (2005)
36. M.P. Kostylev, A.A. Stashkevich, N.A. Sergeeva, Y. Roussigné, J. Magn. Magn. Mater. 278,
397 (2004). doi:10.1016/j.jmmm.2003.11.400
Be the first to comment